#------------------------------------------------------------------------------
#$Date: 2016-02-20 05:06:23 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176774 $
#$URL: svn://www.crystallography.net/cod/cif/2/20/76/2207685.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2207685
loop_
_publ_author_name
'Demchenko, G.'
'Kończyk, J.'
'Demchenko, P.'
'Bodak, O.'
'Marciniak, B.'
_publ_section_title
;
 Trierbium nickel trialuminium digermanide, Er₃NiAl₃Ge₂
;
_journal_coeditor_code           WM6111
_journal_issue                   12
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              i273
_journal_page_last               i274
_journal_paper_doi               10.1107/S1600536805036779
_journal_volume                  61
_journal_year                    2005
_chemical_formula_iupac          'Er3 Ni Al3 Ge2'
_chemical_formula_structural     'Er3 Ni Al3 Ge2'
_chemical_formula_sum            'Al3 Er3 Ge2 Ni'
_chemical_formula_weight         786.61
_chemical_name_common            'Trierbium Nickel Trialuminium Digermanide'
_chemical_name_systematic
;
Trialuminium trierbium digermanium nickel
;
_space_group_IT_number           189
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 -2'
_symmetry_space_group_name_H-M   'P -6 2 m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   6.8360(10)
_cell_length_b                   6.8360(10)
_cell_length_c                   4.1480(9)
_cell_measurement_reflns_used    1298
_cell_measurement_temperature    295(2)
_cell_measurement_theta_max      32.32
_cell_measurement_theta_min      4.91
_cell_volume                     167.87(5)
_computing_cell_refinement       'CrysAlis CCD'
_computing_data_collection       'CrysAlis CCD (Oxford Diffraction, 2004)'
_computing_data_reduction        'CrysAlis RED (Oxford Diffraction, 2005)'
_computing_molecular_graphics    'DIAMOND (Brandenburg, 1999)'
_computing_publication_material  SHELXL97
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      295(2)
_diffrn_measured_fraction_theta_full 0.987
_diffrn_measured_fraction_theta_max 0.987
_diffrn_measurement_device_type  'Oxford Diffraction Xcalibur3 CCD'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0621
_diffrn_reflns_av_sigmaI/netI    0.0301
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       3
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_number            1371
_diffrn_reflns_theta_full        32.32
_diffrn_reflns_theta_max         32.32
_diffrn_reflns_theta_min         4.91
_diffrn_standards_decay_%        0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    48.917
_exptl_absorpt_correction_T_max  0.237
_exptl_absorpt_correction_T_min  0.105
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   '(CrysAlis RED; Oxford Diffraction, 2005)'
_exptl_crystal_colour            'metallic light grey'
_exptl_crystal_density_diffrn    7.781
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             335
_exptl_crystal_size_max          0.22
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.03
_refine_diff_density_max         2.979
_refine_diff_density_min         -1.848
_refine_ls_abs_structure_details 'Flack (1983), 93 Friedel pairs'
_refine_ls_abs_structure_Flack   0.09(8)
_refine_ls_extinction_coef       0.012(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL97
_refine_ls_goodness_of_fit_ref   1.208
_refine_ls_matrix_type           full
_refine_ls_number_parameters     14
_refine_ls_number_reflns         244
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.208
_refine_ls_R_factor_all          0.0282
_refine_ls_R_factor_gt           0.0282
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0361P)²+2.9965P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0731
_refine_ls_wR_factor_ref         0.0731
_reflns_number_gt                244
_reflns_number_total             244
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            wm6111.cif
_cod_data_source_block           I
_cod_database_code               2207685
_cod_database_fobs_code          2207685
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x, y, -z'
'-y, x-y, -z'
'-x+y, -x, -z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'y, x, z'
'x-y, -y, z'
'-x, -x+y, z'
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_type_symbol
Er 0.0000 0.40859(11) 0.5000 0.0109(3) Uani d S 1 Er
Ge 0.6667 0.3333 0.0000 0.0112(5) Uani d S 1 Ge
Ni 0.0000 0.0000 0.5000 0.0120(8) Uani d S 1 Ni
Al 0.7666(8) 0.0000 0.0000 0.0073(10) Uani d S 1 Al
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Er Er -0.2586 4.9576 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
Ni Er Ge . 1_455 102.314(15)
Ni Er Ge . 7_556 102.314(15)
Ge Er Ge 1_455 7_556 155.37(3)
Ni Er Ge . 1_456 102.314(15)
Ge Er Ge 1_455 1_456 90.112(16)
Ge Er Ge 7_556 1_456 84.669(15)
Ni Er Ge . 7 102.314(15)
Ge Er Ge 1_455 7 84.669(15)
Ge Er Ge 7_556 7 90.112(16)
Ge Er Ge 1_456 7 155.37(3)
Ni Er Al . 1_455 51.32(7)
Ge Er Al 1_455 1_455 51.83(9)
Ge Er Al 7_556 1_455 152.20(10)
Ge Er Al 1_456 1_455 107.56(8)
Ge Er Al 7 1_455 87.99(5)
Ni Er Al . 3_666 51.32(7)
Ge Er Al 1_455 3_666 152.20(10)
Ge Er Al 7_556 3_666 51.83(9)
Ge Er Al 1_456 3_666 87.99(5)
Ge Er Al 7 3_666 107.56(8)
Al Er Al 1_455 3_666 102.63(15)
Ni Er Al . 3_665 51.32(7)
Ge Er Al 1_455 3_665 87.99(5)
Ge Er Al 7_556 3_665 107.56(8)
Ge Er Al 1_456 3_665 152.20(10)
Ge Er Al 7 3_665 51.83(9)
Al Er Al 1_455 3_665 51.29(19)
Al Er Al 3_666 3_665 81.03(2)
Ni Er Al . 1_456 51.32(7)
Ge Er Al 1_455 1_456 107.56(8)
Ge Er Al 7_556 1_456 87.99(5)
Ge Er Al 1_456 1_456 51.83(9)
Ge Er Al 7 1_456 152.20(10)
Al Er Al 1_455 1_456 81.03(2)
Al Er Al 3_666 1_456 51.3(2)
Al Er Al 3_665 1_456 102.63(15)
Ni Er Al . 2_556 139.72(7)
Ge Er Al 1_455 2_556 107.15(5)
Ge Er Al 7_556 2_556 51.66(4)
Ge Er Al 1_456 2_556 51.66(4)
Ge Er Al 7 2_556 107.15(5)
Al Er Al 1_455 2_556 153.75(9)
Al Er Al 3_666 2_556 93.26(10)
Al Er Al 3_665 2_556 153.75(9)
Al Er Al 1_456 2_556 93.26(10)
Ni Er Al . 2 139.72(7)
Ge Er Al 1_455 2 51.66(4)
Ge Er Al 7_556 2 107.15(5)
Ge Er Al 1_456 2 107.15(5)
Ge Er Al 7 2 51.66(4)
Al Er Al 1_455 2 93.26(10)
Al Er Al 3_666 2 153.75(9)
Al Er Al 3_665 2 93.26(10)
Al Er Al 1_456 2 153.75(9)
Al Er Al 2_556 2 80.55(13)
Ni Er Er . 3_455 77.57(2)
Ge Er Er 1_455 3_455 52.282(6)
Ge Er Er 7_556 3_455 134.714(7)
Ge Er Er 1_456 3_455 52.282(6)
Ge Er Er 7 3_455 134.714(7)
Al Er Er 1_455 3_455 56.14(9)
Al Er Er 3_666 3_455 106.74(11)
Al Er Er 3_665 3_455 106.74(11)
Al Er Er 1_456 3_455 56.14(9)
Al Er Er 2_556 3_455 99.451(18)
Al Er Er 2 3_455 99.451(18)
Al Ge Al . 2_655 120.0
Al Ge Al . 3_665 120.0
Al Ge Al 2_655 3_665 120.0
Al Ge Er . 1_655 69.12(6)
Al Ge Er 2_655 1_655 69.51(6)
Al Ge Er 3_665 1_655 134.943(8)
Al Ge Er . 3_554 69.51(6)
Al Ge Er 2_655 3_554 134.943(8)
Al Ge Er 3_665 3_554 69.12(6)
Er Ge Er 1_655 3_554 138.633(6)
Al Ge Er . 1_654 69.12(6)
Al Ge Er 2_655 1_654 69.51(6)
Al Ge Er 3_665 1_654 134.943(8)
Er Ge Er 1_655 1_654 90.112(16)
Er Ge Er 3_554 1_654 75.436(13)
Al Ge Er . 3 69.51(6)
Al Ge Er 2_655 3 134.943(8)
Al Ge Er 3_665 3 69.12(6)
Er Ge Er 1_655 3 75.436(13)
Er Ge Er 3_554 3 90.112(16)
Er Ge Er 1_654 3 138.633(6)
Al Ge Er . 2_665 134.943(8)
Al Ge Er 2_655 2_665 69.12(6)
Al Ge Er 3_665 2_665 69.51(6)
Er Ge Er 1_655 2_665 75.436(13)
Er Ge Er 3_554 2_665 138.633(6)
Er Ge Er 1_654 2_665 138.633(6)
Er Ge Er 3 2_665 75.436(13)
Al Ge Er . 2_664 134.943(8)
Al Ge Er 2_655 2_664 69.12(6)
Al Ge Er 3_665 2_664 69.51(6)
Er Ge Er 1_655 2_664 138.633(6)
Er Ge Er 3_554 2_664 75.436(13)
Er Ge Er 1_654 2_664 75.436(13)
Er Ge Er 3 2_664 138.633(6)
Er Ge Er 2_665 2_664 90.112(16)
Al Ni Al 3_666 2_545 144.50(8)
Al Ni Al 3_666 1_455 144.50(8)
Al Ni Al 2_545 1_455 63.74(16)
Al Ni Al 3_666 2_546 63.74(16)
Al Ni Al 2_545 2_546 104.9(2)
Al Ni Al 1_455 2_546 144.50(8)
Al Ni Al 3_666 1_456 63.74(16)
Al Ni Al 2_545 1_456 144.50(8)
Al Ni Al 1_455 1_456 104.9(2)
Al Ni Al 2_546 1_456 63.74(16)
Al Ni Al 3_666 3_665 104.9(2)
Al Ni Al 2_545 3_665 63.74(16)
Al Ni Al 1_455 3_665 63.74(16)
Al Ni Al 2_546 3_665 144.50(8)
Al Ni Al 1_456 3_665 144.50(8)
Al Ni Er 3_666 2 127.57(10)
Al Ni Er 2_545 2 72.25(4)
Al Ni Er 1_455 2 72.25(4)
Al Ni Er 2_546 2 72.25(4)
Al Ni Er 1_456 2 72.25(4)
Al Ni Er 3_665 2 127.57(10)
Al Ni Er 3_666 3 72.25(4)
Al Ni Er 2_545 3 72.25(4)
Al Ni Er 1_455 3 127.57(10)
Al Ni Er 2_546 3 72.25(4)
Al Ni Er 1_456 3 127.57(10)
Al Ni Er 3_665 3 72.25(4)
Er Ni Er 2 3 120.0
Al Ni Er 3_666 . 72.25(4)
Al Ni Er 2_545 . 127.57(10)
Al Ni Er 1_455 . 72.25(4)
Al Ni Er 2_546 . 127.57(10)
Al Ni Er 1_456 . 72.25(4)
Al Ni Er 3_665 . 72.25(4)
Er Ni Er 2 . 120.0
Er Ni Er 3 . 120.0
Ni Al Ni 1_655 1_654 104.9(2)
Ni Al Ge 1_655 . 114.436(15)
Ni Al Ge 1_654 . 114.436(15)
Ni Al Ge 1_655 7_545 114.436(15)
Ni Al Ge 1_654 7_545 114.436(15)
Ge Al Ge . 7_545 94.55(18)
Ni Al Al 1_655 3_765 58.13(8)
Ni Al Al 1_654 3_765 58.13(8)
Ge Al Al . 3_765 102.73(9)
Ge Al Al 7_545 3_765 162.73(9)
Ni Al Al 1_655 2_645 58.13(8)
Ni Al Al 1_654 2_645 58.13(8)
Ge Al Al . 2_645 162.73(9)
Ge Al Al 7_545 2_645 102.73(9)
Al Al Al 3_765 2_645 60.0
Ni Al Er 1_655 1_655 56.43(3)
Ni Al Er 1_654 1_655 118.49(13)
Ge Al Er . 1_655 59.05(3)
Ge Al Er 7_545 1_655 126.79(14)
Al Al Er 3_765 1_655 64.36(10)
Al Al Er 2_645 1_655 108.96(10)
Ni Al Er 1_655 2_654 118.49(13)
Ni Al Er 1_654 2_654 56.43(3)
Ge Al Er . 2_654 126.79(14)
Ge Al Er 7_545 2_654 59.05(3)
Al Al Er 3_765 2_654 108.96(10)
Al Al Er 2_645 2_654 64.36(10)
Er Al Er 1_655 2_654 172.9(2)
Ni Al Er 1_655 1_654 118.49(13)
Ni Al Er 1_654 1_654 56.43(3)
Ge Al Er . 1_654 59.05(3)
Ge Al Er 7_545 1_654 126.79(14)
Al Al Er 3_765 1_654 64.36(10)
Al Al Er 2_645 1_654 108.96(10)
Er Al Er 1_655 1_654 81.03(2)
Er Al Er 2_654 1_654 98.52(3)
Ni Al Er 1_655 2_655 56.43(3)
Ni Al Er 1_654 2_655 118.49(13)
Ge Al Er . 2_655 126.79(14)
Ge Al Er 7_545 2_655 59.05(3)
Al Al Er 3_765 2_655 108.96(10)
Al Al Er 2_645 2_655 64.36(10)
Er Al Er 1_655 2_655 98.52(3)
Er Al Er 2_654 2_655 81.03(2)
Er Al Er 1_654 2_655 172.9(2)
Ni Al Er 1_655 3_554 167.84(17)
Ni Al Er 1_654 3_554 87.29(4)
Ge Al Er . 3_554 58.83(9)
Ge Al Er 7_545 3_554 58.83(9)
Al Al Er 3_765 3_554 131.35(5)
Al Al Er 2_645 3_554 131.35(5)
Er Al Er 1_655 3_554 117.87(12)
Er Al Er 2_654 3_554 68.13(5)
Er Al Er 1_654 3_554 68.13(5)
Er Al Er 2_655 3_554 117.87(12)
Ni Al Er 1_655 3 87.29(4)
Ni Al Er 1_654 3 167.84(17)
Ge Al Er . 3 58.83(9)
Ge Al Er 7_545 3 58.83(9)
Al Al Er 3_765 3 131.35(5)
Al Al Er 2_645 3 131.35(5)
Er Al Er 1_655 3 68.13(5)
Er Al Er 2_654 3 117.87(12)
Er Al Er 1_654 3 117.87(12)
Er Al Er 2_655 3 68.13(5)
Er Al Er 3_554 3 80.55(13)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Er Ni . 2.7931(9) y
Er Ge 1_455 2.9302(4) y
Er Ge 7_556 2.9302(4) ?
Er Ge 1_456 2.9302(4) ?
Er Ge 7 2.9302(4) ?
Er Al 1_455 3.1925(7) y
Er Al 3_666 3.193(4) ?
Er Al 3_665 3.193(4) ?
Er Al 1_456 3.1925(7) ?
Er Al 2_556 3.208(4) y
Er Al 2 3.208(4) ?
Er Er 3_455 3.5853(7) y
Ge Al . 2.686(4) y
Ge Al 2_655 2.686(4) ?
Ge Al 3_665 2.686(4) ?
Ge Er 1_655 2.9302(4) ?
Ge Er 3_554 2.9302(4) ?
Ge Er 1_654 2.9302(4) ?
Ge Er 3 2.9302(4) ?
Ge Er 2_665 2.9302(4) ?
Ge Er 2_664 2.9302(4) ?
Ni Al 3_666 2.617(4) y
Ni Al 2_545 2.617(4) ?
Ni Al 1_455 2.617(4) ?
Ni Al 2_546 2.617(4) ?
Ni Al 1_456 2.617(4) ?
Ni Al 3_665 2.617(4) ?
Ni Er 2 2.7931(9) ?
Ni Er 3 2.7931(9) ?
Al Ni 1_655 2.617(4) ?
Al Ni 1_654 2.617(4) ?
Al Ge 7_545 2.686(4) ?
Al Al 3_765 2.763(10) y
Al Al 2_645 2.763(10) ?
Al Er 1_655 3.1925(7) ?
Al Er 2_654 3.1925(7) ?
Al Er 1_654 3.1925(7) ?
Al Er 2_655 3.1925(7) ?
Al Er 3_554 3.208(4) ?
Al Er 3 3.208(4) ?
